# Manifested flatness defect prediction

date post

16-Oct-2021Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of Manifested flatness defect prediction

Manifested flatness defect predictionSubmitted on 23 Dec 2015

HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.

Manifested flatness defect prediction in cold rolling of thin strips

Rebecca Nakhoul, Pierre Montmitonnet, Nicolas Legrand

To cite this version: Rebecca Nakhoul, Pierre Montmitonnet, Nicolas Legrand. Manifested flatness defect prediction in cold rolling of thin strips. International Journal of Material Forming, Springer Verlag, 2015, 8 (2), pp.283-292. 10.1007/s12289-014-1166-y. hal-00960137

R. Nakhoul a, P. Montmitonnet a, N. Legrand b

a CEMEF, MINES ParisTech, UMR CNRS 7635

Rue Claude Daunesse, CS 10207, 06904 Sophia-Antipolis, France,

[email protected]

[email protected]

Voie Romaine, BP 30320, 57283 Maizières-les-Metz, France

[email protected]

Rue Claude Daunesse, CS 10207, 06904 Sophia-Antipolis Cedex, France

Phone: +33 4 93 95 74 14 Fax : +33 4 93 38 97 52

E-mail : [email protected]

from which heterogeneous strip plastic deformation results. When flatness defects manifest

on line, buckling reorganizes the stress field in the pre- and post-bite areas. Comparison with

flatness roll measurement requires this effect to be taken into account. A coupled Finite

Element Method (FEM) approach is used here to compute stresses and strains in-bite as well

as out-of-bite. The detection of buckled (non-flat) areas is demonstrated for a very thin strip

cold rolling case (“double reduction”). The model is then applied here to two questions,

namely the impact on flatness of the heterogeneous temperature field and the effect of friction

on optimal setting of a flatness actuator, Work Roll Bending.

Keywords: Rolling; Thin Strips; Finite Element Method; Friction; Flatness Defect; Sheet

Buckling; Residual Stress

1. INTRODUCTION

In strip rolling, due to rolls elastic deformation combined with roll grinding crown, thermal

crown and wear, the roll gap is not uniform in the width direction, so that strip reduction

depends on the width coordinate y. Heterogeneous reduction induces residual stresses, and

compressive residual stresses induce buckling (out of plane waviness) if the strip is thin hence

easy to bend. Most of the time, the strip tension is high enough to keep the in-plane stress

tensile everywhere and avoid buckling on-line. But once the strip tension is relaxed, or the

sheet is cut, residual stresses may induce distortions called latent flatness defects, i.e. non

developable, out-of-plane displacements forming periodic waves (centre waves, edge

waves…).

Fig. 1 Schematic view of flatness defects. Note reference frame : x = Rolling Direction (RD),

y = Transverse Direction (TD), z = Normal Direction (ND)

4

However, in some severe operations such as thin strip cold rolling, strain and stress

heterogeneity is exacerbated and on-line strip tension may be insufficient to prevent – or hide

- waviness. In such a case, manifested flatness defects may show on-line (Fig. 1).

If defects are only latent, the stress field computed beyond the bite by e.g. a 3D FEM should

be correct and consistent with measurements. Buckling upon unloading the strip tension can

then be dealt with in an uncoupled way, transferring the stress pattern computed by the rolling

model into a buckling model (e.g. shell FEM). The latter then tells if the critical conditions

for buckling are met, and in this case computes post-buckling mode, wavelength and

amplitude.

On the other hand, it is well known that buckling completely transforms stress fields since the

local stiffness of a buckled sheet drops dramatically. Therefore, if defects are manifested on-

line as is most of the time the case for very thin sheets, the solution coming out of the 3D

FEM of rolling is completely irrelevant outside of the roll bite. Abdelkhalek et al. [1] have

developed a fully coupled buckling model in an implicit finite element software devoted to

rolling processes. They showed that it makes it possible to correct the out-of-bite stress fields

and to come out with values consistent with the σxx(y) profile measurement by a flatness roll.

The question of the impact of this stress reorganization on the strains and stresses within the

bite has also been raised in the same paper. The conclusion is that to the possible exception of

temper-rolling, the feedback effect is very small: the out-of-bite stress rearrangement is

screened by the immediate bite exit area where complex velocity profile changes take place

elastically. In the present paper, it is first recalled how the coupled buckling criterion detects

buckled areas. Then applications to practical questions are examined, such as the setting of a

flatness actuator (work roll bending), the effect of friction on the stress profile and on the

“optimal” work roll bending setting, and the effect of a usual model simplification, isothermal

versus thermally coupled.

2. BRIEF LITERATURE SURVEY

A number of uncoupled models of flatness defects have been presented in the literature. They

are based on the standard solution by Timoshenko and Woinovsky-Krieger of Von Karman’s

equations for a rectangular plate under compressive stress on simply supported edges.

Timoshenko and Woinovsky-Krieger [2] assumed homogeneous stress and sinusoidal waves

in both x and y directions. Bush et al. for instance [3] extended this solution to the complex

fields of strip rolling, allowing only right/left symmetric waves. But as real waves are often

anti-symmetric, Fischer and coworkers [4] chose for the transverse shape either an odd or an

even polynomial in y, while keeping the waves sinusoidal in the rolling direction.

Only the longitudinal stress component (σxx) was used in these papers. Yet, it is easy to see

that not all flatness defects can be handled with this assumption (herringbone defects for

instance are excluded). Moreover, the type of defect (centre or edge wave) was determined by

these authors a priori from the shape of the stress profile, and ad hoc clamping conditions

were applied to get it in the end, to avoid managing too many modes with very similar

energies. On the contrary, Yukawa and coworkers [5] addressed more complete

configurations using shell FEM, again with a non-coupled approach. The bifurcation point

was detected as the load parameter making the second variation of the total elastic strain

energy (i.e. the stiffness matrix) non definite positive. Post-buckling was computed by

introducing a small defect corresponding to the mode, the load step being controlled by a

modified Riks method. This is the standard approach of instabilities in structural mechanics.

Abdelkhalek et al. [6] also proposed a decoupled approach, importing a FEM-computed stress

field in a shell FEM for more generality. In the bifurcation detection stage, they maximized

the load step and decreased the computational burden by managing the loading steps by the

Asymptotic Numerical Method (ANM) developed initially by Zahrouni et al. [7] and

6

improved by Boutyour et al. [8]. ANM consists in developing the solution (displacement and

load parameter) in a power series with respect to a step length parameter, up to a truncation

order p. This series is inserted in the non linear equations of the problem, the different orders

are identified, giving p linear systems with the same stiffness matrix, the right-hand sides of

which are computed from the solutions at lower orders. With this approach, they modelled

both on-line shape (under strip tension) and relaxed shape (strip tensions relieved), whereas

the previous papers dealt only with the latter.

Counhaye [9] was the first who questioned the decoupling of the rolling and the buckling

model. Indeed, buckling sets a limit to the allowable compressive stresses: wherever buckling

occurs, the loss of rigidity changes the stress locally and global changes occur as the stress

field is re-equilibrated. This thorough stress rearrangement on the one hand questions the

stress fields obtained from the rolling models, on the other hand might have an impact even

on in-bite stress and strain fields, or on roll deformation in strongly coupled cases. Therefore,

Counhaye used an approach similar to the one proposed by Roddeman and coworkers [10],

considering buckling as one more strain rate component, present only in the out-of-bite areas,

to be added to the elastic / plastic strain rate splitting. This extra strain rate may be interpreted

as the local shortening of a material segment as it becomes wavy due to buckling.

The model presented in [1] and used here is an adaptation of Counhaye’s model.

7

3. COUPLED ROLL - STRIP ROLLING MODEL WITH EMBEDDED BUCKLING

The model has been presented in details elsewhere previously, so that only general lines will

be recalled hereafter.

3.1 Sheet Rolling model Lam3/Tec3

The rolling model is Lam3/Tec3, a 3D strip / roll stack deformation software developed by

Hacquin and coworkers [11]. The strip elastic-viscoplastic (EVP) deformation is dealt with by

an implicit FEM with a velocity formulation using P1-discretisation on hexahedra. A steady

state formulation based on streamlines is implemented. This requires integrating elastic-

viscoplastic constitutive equations along streamlines determined from the velocity field. In

[12], they described the heterogeneous time step strategy used for this purpose, called

ELDTH (Eulerian-Lagrangian with DT Heterogeneous). In [13], they focused on the semi-

analytical thermo-elastic roll deformation model. Inspired by the work of Berger et al. [14] on

the deformation of a cylinder under complex loadings, Hacquin modelled the roll stack

thermo-elastic deformation based on Timoshenko beam theory (bending component),

Boussinesq solution of a half-space under general loading (flattening part), and Hertz contact

mechanics between work rolls and back-up rolls. These analytical approaches were found

insufficient near the roll barrel edge, therefore edge effects were corrected by analytical

functions calibrated using an extensive FEM roll deformation campaign under various

geometries and loading conditions [11,13].

Equations are discretized by an influence function method (IFM). Writing the global

equilibrium of the roll stack under the combined effects of the roll – strip contact stresses,

external (roll load) and internal (e.g. roll bending) forces, a system of equations is found, the

unknowns of which are the roll rigid body displacement, contact line displacement field and

8

contact pressure profiles at work roll / back-up roll and work roll / strip contact. This system,

non-linear due to unknown contact lines, is solved by Newton-Raphson method.

Both strip and roll temperatures are computed and coupled with mechanics. The strip

temperature model uses a straightforward 3D SUPG (Streamline-Upwind Petrov Galerkin)

Finite Element scheme. The roll temperature (and roll crown) model is a combination of 2D

(r,θ) and (r,z) FEM coordinated by another influence function technique. Details and

validation can be found in [11].

In [15], the whole roll stack deformation model was validated under isothermal conditions

against experimental measurements performed under diverse loading conditions. Later on in

[16], a successful numerical comparison was carried out with the model of Yanagimoto and

Kiuchi [17], which uses a beam bending model for roll bending and 3D FEM for flattening,

and with the model of Kim et al. [18] where full 3D elastic FEM is used for roll stack

deformation and strip deformation altogether; all three models were compared with the

experiments reported by [17]. Therefore, this roll stack deformation model, essential for strip

flatness, can be used with confidence for the purpose of the present paper.

3.2 Simple buckling model embedded in Lam3/Tec3

Counhaye’s model [9] has been implemented in Lam3/Tec3 [1]. Initially proposed within the

membrane theory framework in [10], it forbids the appearance of a negative stress:

everywhere compression is about to occur, the structure buckles, bringing the stress back to

almost zero by providing a stress-free alternative to elastic shortening of a material line. The

following critical conditions are introduced:

0.. 0.. 0..

(1)

9

where 1n and 2n are the principal directions of the Cauchy stress tensor σ in the buckled

structure (hence the third equation). Principal directions are determined first, and the angle

they make with (x,y) is called α. When a tension is applied in a direction (here 2n ), the

membrane is stiff; if the stress becomes negative, it gets slack and in fact, the corresponding

stress is put to 0 (direction 1n ). The essence of the model consists in determining an extra

deformation which elastically brings the stress in the buckled direction back to 0. It may be

interpreted as the shortening of a material line due to buckling of the structure. This is more

or less analogous to elastic-plastic decomposition, but is activated only out of the roll bite, i.e.

where buckling is liable to occur:

buel εεε += (2)

εel is the elastic and εbu is the “buckling strain” increment. Plane stress is assumed outside

of the roll bite. The extra deformation representing buckling is computed in the principal axes,

and then transported to the reference frame. Let λi, i = I, II, be the principal components of

this extra strain. It is deduced from σi, i = I, II as follows:

IIIi E

ci i ,=

σσ λ (3)

Moving back to the reference frame (Oxyz), the buckling strain increment is added to the

global strain increment. In the following equation, u and v are the two in-plane incremental

10

displacements, α is the angle between principal and reference frames in the plane of the strip,

ν is Poisson's ratio and E is Young's modulus:

( )yyxxzz

IIIxy

IIIyy

IIIxx

sin.cos.

sin.cos.

22

22

(4)

This strain increment replaces the standard one fed into the module which solves the

constitutive differential equations.

4.1 Definition of rolls, material, strip dimensions

All examples and parametric studies described hereafter refer to the same rolling pass, the last

stand of a tinplate sheet mill, with very low thickness. All the characteristics are given in

Table 1, together with the stress-strain curve:

( ) (MPa) 175))9.8exp(.45.01(.4.1755.4700 −−−×+= εεσ (5)

σ0 is the yield stress in tension, ε is the equivalent plastic strain. Coulomb friction is

assumed, the friction coefficient is µ = 0.03 unless otherwise stated.

11

Strip width 855 mm

Strip thickness (strip crown)

0.355 mm (4.81 %)

Exit thickness 0.252 mm Rolling speed 22 m/s Front / back tension

100 MPa / 170 MPa

Type of mill Work rolls diameter Backup rolls diameter Work rolls length Backup rolls length

4-high 555mm 1300mm 1400mm 1295mm

Work rolls crown Backup rolls crown

0.0322 % No crown

Screw force application point y = 1075 mm

Friction law 0, 03 nτ σ= × Young’s modulus Poisson’s ratio

E = 210 GPa ν = 0.3

4.2 Roll and strip deformation leading to buckling

The roll load profile F(y) computed by the coupled roll / strip deformation model is pictured

in Fig. 2a, together with the resulting shape of the deformed roll generator (Fig. 2b). By the

way, Fig. 2b illustrates the very weak effect of coupling or not buckling on these in-bite

characteristics.

The work roll shape displays a large flattening component, of the order of 0.07 mm. The

bending component shows outside the work roll / strip contact (i.e. y > 430 mm), and is partly

hidden in the contact area by flattening. The roll load profiles display distinct peaks near the

edge of the strip for the work roll and at the edge of the work roll for the backup roll. The

peak of the work roll load profile is explained by Fig. 3, which shows that the reduction, from

a nominal, central 29%, reaches 50% at the very edge of the strip, with a significantly longer

bite.

12

0

2000

4000

6000

8000

10000

12000

14000

16000

F( y)

(k N

y (mm)

Zr ol

l ( m

Fig. 2 Coupled deformation of strip and roll:

(a) work roll (WR) and backup roll (BUR) load profiles F(y)

(b) roll generator shape, comparing calculations with / without accounting for strip buckling

0,15

0,17

0,19

0,21

0,23

0,25

0,27

0 50 100 150 200 250 300 350 400 450

Width coordinate y (mm)

0 50 100 150 200 250 300 350 400 450

Width coordinate y (mm)

Th ic

kn es

s re

du ct

io n

(a) (b)

Fig. 3 Strain heterogeneity. (a) comparison of inlet and exit strip thickness profiles. (b) the

thickness reduction profile

4.3 Impact of buckling being accounted for

With a reservation for very small reduction (temper-rolling), it has been found that this

rearrangement of out-of-bite stress has significant impact neither on strain and stress fields in

13

the bite, nor on the roll loads and deformation [1]. Neglecting buckling is therefore licit if

only the behaviour in the bite is to be studied.

Fig. 4 Comparison of the experimental and numerical σxx(y) stress profiles, ≈ 1 m after roll

bite exit

But the “residual” stress field in the strip, under these conditions, is very far from the flatness

roll measurement, as shown in Fig. 4. “Residual” means here post-bite, on-line under tension.

The measurements (dots) show an almost flat stress profile (at the scale of the drawing). FEM

results without buckling (dashed line) give an enormous compressive stress at the edge, due

to a very large elongation gradient connected with roll flattening and the edge drop defect

(see Fig. 3). This very high compressive stress is compensated for by a high tensile stress in

the centre, since the resultant must be equal to the sheet tension force (here given by the

tension stress of 100 MPa, Table 1). Also to be noted is a stress peak at y ≈ 415 mm (i.e. ca.

10 mm from strip edge). It is much more conspicuous when buckling relaxes partly the stress

14

(as in figure 8 or 12); the same location and amplitude is found whatever the mesh size; it is

in fact exactly at the location where the edge-drop starts, i.e. the transition between the

flattened and free zones of the roll profile, see figure 2b.

When buckling is accounted for, i.e. equations (1-4) are activated, the computed stress profile

(full line) comes close to the experiments. More details can be found in the authors’ previous

paper [1]. Therefore, for out-of-bite stress prediction and comparison with stress-meter

measurements, accounting for buckling is essential, at least for thin strips.

a b

Fig. 5 σxx stress maps at the edge, in the vicinity of the roll bite. a - without buckling

computation. b - with buckling computation. Rolling direction Ox is vertical, upward.

Fig. 5 shows the σxx stress map at the edge, slightly before and slightly after the roll bite, i.e.

far ahead of the location of the profiles of Fig. 4. It compares computations without (Fig. 5a)

and with (Fig. 5b) the buckling model. The stress is very much compressive in the bite as

15

expected. In the latter case, a thorough reorganization of the stress pattern just after bite exit

results in the stress being relaxed to almost zero on the edge within 20 – 30 mm from bite exit,

instead of dropping abruptly to -1200 MPa.

a b

Fig. 6 « Buckling strain » principal components: a - λI (corresponding to σxx stress); b - λII

(corresponding to a σyy stress)

Fig. 6 maps the λi’s in the same area. It is found that the reference and principal stress frames

coincide almost everywhere, i.e. α = 0, except for small high shear zones at the edge on either

sides of the roll bite. Hence λI ≠ 0 corresponds to a x-wave (wavy edge) and λΙΙ ≠ 0 to y-wave,

the so-called “towel effect”. Whereas the former is moving with the strip and constitutes a

real flatness defect, the latter is a stationary phenomenon which can be observed sometimes at

the exit of the bite. It is due to a flexible membrane being submitted to a tension under a non-

strictly homogeneous tension stress (e.g. due to the clamping effect of the roll bite). It has no

practical consequences for the strip most of the time, except if it becomes so large that double

thickness rolling occurs; this improbable case is not addressed here.

16

Both types of waves are detected by the model. It should be emphasized, though, that the

present buckling model is embedded in a steady state rolling model, so that it represents a

moving defect in a stationary context. It can therefore detect wave formation, but not

characterize its geometry.

5. FIRST APPLICATION: IMPACT OF TEMPERATURE FIELD ON FLATNESS

Most of the time, thermal effects are neglected in steel cold rolling, and flatness defects are

studied under isothermal conditions. Here, with all three couplings available: strip – roll,

mechanical - thermal, and buckling, many effects may be investigated.

Indeed, at bite exit, the temperature is much larger at the edge than in the centre (Fig. 7),

about 438 K (165°C) versus 383 K (110°C). This is due to larger reduction and plastic

heating (see Fig. 3). Due to the corresponding differential dilatation, the post-bite stress

pattern could be affected. A series of simulations has therefore been run, with roll

temperature calculated at steady state (i.e. after a long rolling time). The isothermal case is

taken as a reference. In the second case, the strip is allowed to cool after bite exit under the

effect of the strip cooling system, with heat transfer coefficient (HTC) Hcool = 5 kW.m-2.K-1 ;

strip - roll contact is kept adiabatic (Hroll = 0). Temperature increases in the roll bite and

slowly decays afterwards (remember 1 m ≈ 0.05 s). In the third case, the roll - strip interface

is represented by Hroll = 100 kW.m-2.K-1. The temperature increase is less in the bite, cooling

is similar to the previous case. Finally, in the fourth case, Hcool = 5 kW.m-2.K-1, Hroll = 100

kW.m-2.K-1, but rolls are moreover cooled efficiently by water sprays, so that strip

temperatures are significantly lower.

Yet, the temperature difference between strip edge and centre is very similar in all 3 cases,

313 to 323 K (40°C to 50°C). Fig. 8 shows that these temperature differences, even in the

17

isothermal case (T = 298 K or 25°C everywhere), have negligible impact on the stress pattern

once relaxed by edge buckling.

Fig. 7 Effect of thermal boundary conditions on central and edge longitudinal temperature

profiles in the rolled strip. Top: long range post-bite evolution. Bottom: detail of plastic

heating in the roll bite

18

Fig. 8 Effect of all thermal boundary conditions on stress transverse profile, σxx(y)

6. FRICTION-SENSITIVE SETTING OF WORK ROLL BENDING FORCES

Work roll bending is a typical sheet profile and flatness actuator: by applying a torque

opposed to the contact stress moment, rolls are brought closer to their rest shape. This is a

more flexible actuator than e.g. roll crown, which is chosen and fixed for a whole roll

mounting. The work roll bending force can be controlled by monitoring the post-bite strip

stress profile by a flatness roll, to answer variations in rolling conditions. Such variations

often come from friction which may fluctuate due to (i) progressive roll roughness wear from

coil to coil or (ii) accelerations and decelerations at coil beginning and end. Jiang and co-

workers have proved in [19] that friction impacts strip profile after cold rolling and

demonstrated the effect of a parabolic variation of friction in the transverse direction in [20].

It is therefore important to quantify the effects of such friction time variations. Friction is

assumed homogeneous here.

6.1 Impact of friction on roll deformation

Figs. 9-12 illustrate a parametric study whereby friction varies between µ = 0.01 (slight

skidding) and µ = 0.035. The impact on roll deformation under a fixed work roll bending

force of 482 kN is first shown. Low friction gives a low rolling load (Fig. 9), and moderate

roll deformation (Fig. 10). The shape of the work roll generator therefore mainly corresponds

to counter-bending by the work roll bending force.

Fig. 9 Effect of varying friction on the work rolls load profile F(y). Work roll bending force

is equal to 482 kN

At µ = 0.035, the rolling load is very high (compare the work roll load profiles), so that roll

kiss occurs (work rolls touch each other on either sides of the strip). The resulting strip

thickness profiles show differences (a few µm) which may look small, but are very important

in terms of residual stress and flatness. The latter are pictured in Fig. 12: µ = 0.01 gives

strong tension on edges and slack centre (wavy centre), whereas the stress profile is most flat

when µ = 0.03, leaving just a few mm of slack metal near the edges, with a probable small

size wavy edge there.

20

Fig. 10 Effect of varying friction on the deformed roll generator shape (bottom). Work roll

bending force is equal to 482 kN

Fig. 11 Effect of varying friction on strip thickness profile (bottom). Work roll bending

force is equal to 482 kN

21

Fig. 12 The impact of friction and transverse profile of strip stress (latent flatness defect).

Work roll bending force is equal to 482 kN

6.2 Impact of work roll bending force at fixed µ

Now, the work roll bending force is varied at constant µ = 0.025 (Fig. 13). The very high

work roll bending force (900 kN) again gives a low, yet positive, stress in the centre, which

will probably result in a wavy centre, at least after tension is cancelled. The most flat stress

profile turns out to be for a work roll bending force equal to 350 kN.

Finally, Fig. 14 summarizes the bending force found “optimal” for each value of the friction

coefficient, i.e. giving the most flat stress profile “by eye”. This graph gives an idea of how to

preset the work roll bending force as a function of varying friction, in the present rolling

operation of Table 1.

22

Fig. 13 The σxx(y) stress profile for varying bending force and fixed friction coefficient µ =

0.025

Fig. 14 The relationship between friction and optimal bending force

23

7. CONCLUSION

The main outcome of the present paper is to show that a simple buckling model can be

coupled to a finite element rolling model and applied to practical questions concerning

flatness in cold strip rolling. In-bite stress and strain are not affected by post-buckling stress

rearrangement, but the residual stress is, in case of manifested defects expected with very thin

strips.

The results presented above suggest that for cold rolling, the heterogeneous temperature field

does not change significantly the stress pattern, which is dominated by the rearrangement of

the stress field as the elastic strain recovery takes place in the immediate post-bite area. This

analysis contributes to shed light on which features of the rolling process may be neglected or

not, depending on the objective: in bite stress and strain, roll deformation and strip crown do

not need particularly buckling to be coupled; the residual state of the strip is very sensitive to

buckling whenever it takes place on-line, but it is not sensitive to thermal transfer.

It has been shown also here that friction has an impact on reduction profile, in particular on

the edge thickness, through roll load distribution and roll deformation. This strongly changes

residual stress distribution when thin strips are dealt with. For a given work roll bending force,

just changing friction may turn the strip shape from flat to wavy edge to wavy centre.

Conversely, for each level of friction, an “optimal” work roll bending force can be proposed

based on results of the model.

The buckling model presented in section 3.2 deals with buckling at material point (or finite

element) level, which is questionable; but it is strongly coupled at constitutive equations level,

which Abdelkhalek et al. have shown to be important for precise residual stress prediction

[21]. It cannot predict the geometry of defects quantitatively. These are serious limitations.

24

Work is in progress to try and implement more physically founded models which give

quantitative information on defect geometry. These efforts will be reported somewhere else.

ACKNOWLEDGEMENT

The authors wish to thank the French National Research Agency (ANR) for its financial

support under Contract ANR – 2010- RMNP-019-01, and the partners of the Platform Project

(ArcelorMittal Maizières research, Constellium CRV, CNRS, CEA, Université de Lorraine,

INSA Lyon and ARMINES) for authorization to publish this work. Particular thanks are due

to M. Potier-Ferry and H. Zahrouni, from LEM3 laboratory, for most helpful discussions.

REFERENCES

1. Abdelkhalek S, Montmitonnet P, Legrand N, Buessler P (2011) Coupled approach for

flatness predictions in thin strip cold rolling. Int. J. Mech. Sci. 53: 651-675

2. Timoshenko S, Woinovsky-Krieger S (1940) Theory of plates and shells, McGraw-Hill

Book Co., New York

3. Bush A, Nicholls R, Tunstall J (2001) Stress levels for elastic buckling of rolled strip

and plate. Ironm. Steelm. 28: 481-484

4. Fisher FD, Rammerstorfer FG, Friedl N, Wisser W (2000) Buckling phenomena related

to rolling and levelling of sheet metal. Int. J. Mech. Sci. 42: 1887-1910

5. Yukawa N, Ishikawa T, Tozawa Y (1986) Numerical analysis of the shape of rolled

strip. In: Proc. NUMIFORM Conference, August 25-29, Gothenburg, Sweden

6. Abdelkhalek S, Zahrouni H, Potier-Ferry M, Montmitonnet P, Legrand N, Buessler P

(2009) Modélisation numérique du flambage des plaques minces et application au

laminage. In : Proc. (CD-ROM) CFM 2009August 24-28, Marseille, France. In French

25

7. Zahrouni H, Cochelin B, Potier-Ferry M (1999) Computing finite rotations of shells by

an Asymptotic-Numerical Method. Comp. Meth. Appl. Mech. Engg 175: 71-85

8. Boutyour EH, Zahrouni H, Potier-Ferry M, Boudi M (2004) Bifurcation points and

bifurcated branches by an Asymptotic Numerical Method and Padé approximants. Int.

J. Num. Meth. Engg, 60: 1987-2012

9. C. Counhaye (2000) Modélisation et contrôle industriel de la géométrie des aciers

laminés à froid. PhD Thesis, Liège University. In French

10. Roddeman DG, Drukker J, Oomens CWJ, Janssen JD (1987) The Wrinkling of Thin

Membranes: Part I-Theory. ASME Trans. J. Appl. Mech. 54: 884-887

11. Hacquin A (1996) Modélisation thermomécanique tridimensionnelle du laminage -

Couplage bande / cylindres (3D thermomechanical model of rolling - Strip-roll

coupling). PhD Thesis, Ecole des Mines de Paris, France. In French.

12. Hacquin A, Montmitonnet P, Guilleraut JP (1998) A steady state thermo-elasto-

viscoplastic finite element model of rolling with coupled thermo-elastic roll

deformation. J. Mat. Proc. Tech. 60: 109-116

13. Hacquin A, Montmitonnet P, Guilleraut JP (1998) A 3D semi-analytical model of

rolling stand deformation with finite element validation. Eur. J. Mech. A (Solids) 17:

79-106

14. Berger B, Pawelski O, Funke B (1976) Die elastische Verformung der Walzen von

Vierwalzengerüsten. Arch. Eisenhüttenwes. 47: 351-356. In German

15. Hacquin A, Montmitonnet P, Guillerault JP (1994) Experimental validation of a Rolling

Stand Elastic Deformation Model, J. Mater. Process. Technol. 45: 199-206

16. Montmitonnet P (2006) Comparison of profile prediction models for strip rolling,

Conference “Achieving Profile & Flatness in Flat Products” Austin Court, Birmingham,

UK

26

17. J. Yanagimoto , M. Kiuchi : 3D simulation system for coupled elastic / rigid plastic

deformation of rolls and workpieces in strip rolling processes. Proc. NUMIFORM 92

(Sophia-Antipolis, France, 1992). J.L. Chenot et al. eds. A.A. Balkema, Rotterdam

(1992)

18. T.H. Kim, W.H. Lee, S.M. Hwang : An integrated FE process model for the prediction

of strip profile in flat rolling. ISIJ Int. 43, 12 (2003) 1947-1956

19. Jiang ZY, Tieu AK, Zhang XM, Lu C, Sun WH (2003) Finite element simulation of

cold rolling of thin strip. J. Mat. Proc. Tech. 140: 542–547

20. Jiang ZY, Xiong SW, Tieu AK, Wang QJ (2008) Modelling of the effect of friction on

cold strip rolling. J. Mat. Proc. Tech. 201: 85-90

21. Abdelkhalek S, Zahrouni H, Montmitonnet P, Legrand N, Potier-Ferry M (2011)

Manifested flatness predictions in thin strip cold rolling using a general rolling FEM

model, Steel Res. Int., Sp. Iss. “ICTP 2011” :111-116

27

Figure captions

Fig. 1 Schematic view of flatness defects. Note reference frame : x = Rolling Direction

(RD), y = Transverse Direction (TD), z = Normal Direction (ND)

Fig. 2 Coupled deformation of strip and roll:

(a) work roll (WR) and backup roll (BUR) load profiles F(y),

(b) roll generator shape, comparing calculations with / without accounting for

strip buckling

Fig. 3 Strain heterogeneity. (a) comparison of inlet and exit strip thickness profiles. (b)

the thickness reduction profile

Fig. 4 Comparison of the experimental and numerical σxx(y) stress profiles, ≈ 1 m after

roll bite exit

Fig. 5 σxx stress maps at the edge, in the vicinity of the roll bite. a - without buckling

computation. b - with buckling computation. Rolling direction Ox is vertical,

upward.

Fig. 6 « Buckling strain » principal components: a - λI (corresponding to σxx stress); b

- λII (corresponding to a σyy stress)

Fig. 7 Effect of thermal boundary conditions on central and edge longitudinal

temperature profiles in the rolled strip. Left: long range post-bite evolution.

Right: detail of plastic heating in the roll bite

Fig. 8 Effect of all thermal boundary conditions on RD stress transverse profile, σxx(y).

Fig. 9 Effect of varying friction on the work rolls load profile F(y). Work roll bending

force is equal to 482 kN

Fig. 10 Effect of varying friction on the deformed roll generator shape (bottom). Work

roll bending force is equal to 482 kN

28

Fig. 11 Effect of varying friction on strip thickness profile (bottom). Work roll bending

force is equal to 482 kN

Fig. 12 The impact of friction and transverse profile of strip stress (latent flatness

defect). Work roll bending force is equal to 482 kN

Fig. 13 The σxx(y) stress profile for varying bending force and fixed µ = 0.025)

Fig. 14 The relationship between friction and optimal bending force

Table caption

HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.

Manifested flatness defect prediction in cold rolling of thin strips

Rebecca Nakhoul, Pierre Montmitonnet, Nicolas Legrand

To cite this version: Rebecca Nakhoul, Pierre Montmitonnet, Nicolas Legrand. Manifested flatness defect prediction in cold rolling of thin strips. International Journal of Material Forming, Springer Verlag, 2015, 8 (2), pp.283-292. 10.1007/s12289-014-1166-y. hal-00960137

R. Nakhoul a, P. Montmitonnet a, N. Legrand b

a CEMEF, MINES ParisTech, UMR CNRS 7635

Rue Claude Daunesse, CS 10207, 06904 Sophia-Antipolis, France,

[email protected]

[email protected]

Voie Romaine, BP 30320, 57283 Maizières-les-Metz, France

[email protected]

Rue Claude Daunesse, CS 10207, 06904 Sophia-Antipolis Cedex, France

Phone: +33 4 93 95 74 14 Fax : +33 4 93 38 97 52

E-mail : [email protected]

from which heterogeneous strip plastic deformation results. When flatness defects manifest

on line, buckling reorganizes the stress field in the pre- and post-bite areas. Comparison with

flatness roll measurement requires this effect to be taken into account. A coupled Finite

Element Method (FEM) approach is used here to compute stresses and strains in-bite as well

as out-of-bite. The detection of buckled (non-flat) areas is demonstrated for a very thin strip

cold rolling case (“double reduction”). The model is then applied here to two questions,

namely the impact on flatness of the heterogeneous temperature field and the effect of friction

on optimal setting of a flatness actuator, Work Roll Bending.

Keywords: Rolling; Thin Strips; Finite Element Method; Friction; Flatness Defect; Sheet

Buckling; Residual Stress

1. INTRODUCTION

In strip rolling, due to rolls elastic deformation combined with roll grinding crown, thermal

crown and wear, the roll gap is not uniform in the width direction, so that strip reduction

depends on the width coordinate y. Heterogeneous reduction induces residual stresses, and

compressive residual stresses induce buckling (out of plane waviness) if the strip is thin hence

easy to bend. Most of the time, the strip tension is high enough to keep the in-plane stress

tensile everywhere and avoid buckling on-line. But once the strip tension is relaxed, or the

sheet is cut, residual stresses may induce distortions called latent flatness defects, i.e. non

developable, out-of-plane displacements forming periodic waves (centre waves, edge

waves…).

Fig. 1 Schematic view of flatness defects. Note reference frame : x = Rolling Direction (RD),

y = Transverse Direction (TD), z = Normal Direction (ND)

4

However, in some severe operations such as thin strip cold rolling, strain and stress

heterogeneity is exacerbated and on-line strip tension may be insufficient to prevent – or hide

- waviness. In such a case, manifested flatness defects may show on-line (Fig. 1).

If defects are only latent, the stress field computed beyond the bite by e.g. a 3D FEM should

be correct and consistent with measurements. Buckling upon unloading the strip tension can

then be dealt with in an uncoupled way, transferring the stress pattern computed by the rolling

model into a buckling model (e.g. shell FEM). The latter then tells if the critical conditions

for buckling are met, and in this case computes post-buckling mode, wavelength and

amplitude.

On the other hand, it is well known that buckling completely transforms stress fields since the

local stiffness of a buckled sheet drops dramatically. Therefore, if defects are manifested on-

line as is most of the time the case for very thin sheets, the solution coming out of the 3D

FEM of rolling is completely irrelevant outside of the roll bite. Abdelkhalek et al. [1] have

developed a fully coupled buckling model in an implicit finite element software devoted to

rolling processes. They showed that it makes it possible to correct the out-of-bite stress fields

and to come out with values consistent with the σxx(y) profile measurement by a flatness roll.

The question of the impact of this stress reorganization on the strains and stresses within the

bite has also been raised in the same paper. The conclusion is that to the possible exception of

temper-rolling, the feedback effect is very small: the out-of-bite stress rearrangement is

screened by the immediate bite exit area where complex velocity profile changes take place

elastically. In the present paper, it is first recalled how the coupled buckling criterion detects

buckled areas. Then applications to practical questions are examined, such as the setting of a

flatness actuator (work roll bending), the effect of friction on the stress profile and on the

“optimal” work roll bending setting, and the effect of a usual model simplification, isothermal

versus thermally coupled.

2. BRIEF LITERATURE SURVEY

A number of uncoupled models of flatness defects have been presented in the literature. They

are based on the standard solution by Timoshenko and Woinovsky-Krieger of Von Karman’s

equations for a rectangular plate under compressive stress on simply supported edges.

Timoshenko and Woinovsky-Krieger [2] assumed homogeneous stress and sinusoidal waves

in both x and y directions. Bush et al. for instance [3] extended this solution to the complex

fields of strip rolling, allowing only right/left symmetric waves. But as real waves are often

anti-symmetric, Fischer and coworkers [4] chose for the transverse shape either an odd or an

even polynomial in y, while keeping the waves sinusoidal in the rolling direction.

Only the longitudinal stress component (σxx) was used in these papers. Yet, it is easy to see

that not all flatness defects can be handled with this assumption (herringbone defects for

instance are excluded). Moreover, the type of defect (centre or edge wave) was determined by

these authors a priori from the shape of the stress profile, and ad hoc clamping conditions

were applied to get it in the end, to avoid managing too many modes with very similar

energies. On the contrary, Yukawa and coworkers [5] addressed more complete

configurations using shell FEM, again with a non-coupled approach. The bifurcation point

was detected as the load parameter making the second variation of the total elastic strain

energy (i.e. the stiffness matrix) non definite positive. Post-buckling was computed by

introducing a small defect corresponding to the mode, the load step being controlled by a

modified Riks method. This is the standard approach of instabilities in structural mechanics.

Abdelkhalek et al. [6] also proposed a decoupled approach, importing a FEM-computed stress

field in a shell FEM for more generality. In the bifurcation detection stage, they maximized

the load step and decreased the computational burden by managing the loading steps by the

Asymptotic Numerical Method (ANM) developed initially by Zahrouni et al. [7] and

6

improved by Boutyour et al. [8]. ANM consists in developing the solution (displacement and

load parameter) in a power series with respect to a step length parameter, up to a truncation

order p. This series is inserted in the non linear equations of the problem, the different orders

are identified, giving p linear systems with the same stiffness matrix, the right-hand sides of

which are computed from the solutions at lower orders. With this approach, they modelled

both on-line shape (under strip tension) and relaxed shape (strip tensions relieved), whereas

the previous papers dealt only with the latter.

Counhaye [9] was the first who questioned the decoupling of the rolling and the buckling

model. Indeed, buckling sets a limit to the allowable compressive stresses: wherever buckling

occurs, the loss of rigidity changes the stress locally and global changes occur as the stress

field is re-equilibrated. This thorough stress rearrangement on the one hand questions the

stress fields obtained from the rolling models, on the other hand might have an impact even

on in-bite stress and strain fields, or on roll deformation in strongly coupled cases. Therefore,

Counhaye used an approach similar to the one proposed by Roddeman and coworkers [10],

considering buckling as one more strain rate component, present only in the out-of-bite areas,

to be added to the elastic / plastic strain rate splitting. This extra strain rate may be interpreted

as the local shortening of a material segment as it becomes wavy due to buckling.

The model presented in [1] and used here is an adaptation of Counhaye’s model.

7

3. COUPLED ROLL - STRIP ROLLING MODEL WITH EMBEDDED BUCKLING

The model has been presented in details elsewhere previously, so that only general lines will

be recalled hereafter.

3.1 Sheet Rolling model Lam3/Tec3

The rolling model is Lam3/Tec3, a 3D strip / roll stack deformation software developed by

Hacquin and coworkers [11]. The strip elastic-viscoplastic (EVP) deformation is dealt with by

an implicit FEM with a velocity formulation using P1-discretisation on hexahedra. A steady

state formulation based on streamlines is implemented. This requires integrating elastic-

viscoplastic constitutive equations along streamlines determined from the velocity field. In

[12], they described the heterogeneous time step strategy used for this purpose, called

ELDTH (Eulerian-Lagrangian with DT Heterogeneous). In [13], they focused on the semi-

analytical thermo-elastic roll deformation model. Inspired by the work of Berger et al. [14] on

the deformation of a cylinder under complex loadings, Hacquin modelled the roll stack

thermo-elastic deformation based on Timoshenko beam theory (bending component),

Boussinesq solution of a half-space under general loading (flattening part), and Hertz contact

mechanics between work rolls and back-up rolls. These analytical approaches were found

insufficient near the roll barrel edge, therefore edge effects were corrected by analytical

functions calibrated using an extensive FEM roll deformation campaign under various

geometries and loading conditions [11,13].

Equations are discretized by an influence function method (IFM). Writing the global

equilibrium of the roll stack under the combined effects of the roll – strip contact stresses,

external (roll load) and internal (e.g. roll bending) forces, a system of equations is found, the

unknowns of which are the roll rigid body displacement, contact line displacement field and

8

contact pressure profiles at work roll / back-up roll and work roll / strip contact. This system,

non-linear due to unknown contact lines, is solved by Newton-Raphson method.

Both strip and roll temperatures are computed and coupled with mechanics. The strip

temperature model uses a straightforward 3D SUPG (Streamline-Upwind Petrov Galerkin)

Finite Element scheme. The roll temperature (and roll crown) model is a combination of 2D

(r,θ) and (r,z) FEM coordinated by another influence function technique. Details and

validation can be found in [11].

In [15], the whole roll stack deformation model was validated under isothermal conditions

against experimental measurements performed under diverse loading conditions. Later on in

[16], a successful numerical comparison was carried out with the model of Yanagimoto and

Kiuchi [17], which uses a beam bending model for roll bending and 3D FEM for flattening,

and with the model of Kim et al. [18] where full 3D elastic FEM is used for roll stack

deformation and strip deformation altogether; all three models were compared with the

experiments reported by [17]. Therefore, this roll stack deformation model, essential for strip

flatness, can be used with confidence for the purpose of the present paper.

3.2 Simple buckling model embedded in Lam3/Tec3

Counhaye’s model [9] has been implemented in Lam3/Tec3 [1]. Initially proposed within the

membrane theory framework in [10], it forbids the appearance of a negative stress:

everywhere compression is about to occur, the structure buckles, bringing the stress back to

almost zero by providing a stress-free alternative to elastic shortening of a material line. The

following critical conditions are introduced:

0.. 0.. 0..

(1)

9

where 1n and 2n are the principal directions of the Cauchy stress tensor σ in the buckled

structure (hence the third equation). Principal directions are determined first, and the angle

they make with (x,y) is called α. When a tension is applied in a direction (here 2n ), the

membrane is stiff; if the stress becomes negative, it gets slack and in fact, the corresponding

stress is put to 0 (direction 1n ). The essence of the model consists in determining an extra

deformation which elastically brings the stress in the buckled direction back to 0. It may be

interpreted as the shortening of a material line due to buckling of the structure. This is more

or less analogous to elastic-plastic decomposition, but is activated only out of the roll bite, i.e.

where buckling is liable to occur:

buel εεε += (2)

εel is the elastic and εbu is the “buckling strain” increment. Plane stress is assumed outside

of the roll bite. The extra deformation representing buckling is computed in the principal axes,

and then transported to the reference frame. Let λi, i = I, II, be the principal components of

this extra strain. It is deduced from σi, i = I, II as follows:

IIIi E

ci i ,=

σσ λ (3)

Moving back to the reference frame (Oxyz), the buckling strain increment is added to the

global strain increment. In the following equation, u and v are the two in-plane incremental

10

displacements, α is the angle between principal and reference frames in the plane of the strip,

ν is Poisson's ratio and E is Young's modulus:

( )yyxxzz

IIIxy

IIIyy

IIIxx

sin.cos.

sin.cos.

22

22

(4)

This strain increment replaces the standard one fed into the module which solves the

constitutive differential equations.

4.1 Definition of rolls, material, strip dimensions

All examples and parametric studies described hereafter refer to the same rolling pass, the last

stand of a tinplate sheet mill, with very low thickness. All the characteristics are given in

Table 1, together with the stress-strain curve:

( ) (MPa) 175))9.8exp(.45.01(.4.1755.4700 −−−×+= εεσ (5)

σ0 is the yield stress in tension, ε is the equivalent plastic strain. Coulomb friction is

assumed, the friction coefficient is µ = 0.03 unless otherwise stated.

11

Strip width 855 mm

Strip thickness (strip crown)

0.355 mm (4.81 %)

Exit thickness 0.252 mm Rolling speed 22 m/s Front / back tension

100 MPa / 170 MPa

Type of mill Work rolls diameter Backup rolls diameter Work rolls length Backup rolls length

4-high 555mm 1300mm 1400mm 1295mm

Work rolls crown Backup rolls crown

0.0322 % No crown

Screw force application point y = 1075 mm

Friction law 0, 03 nτ σ= × Young’s modulus Poisson’s ratio

E = 210 GPa ν = 0.3

4.2 Roll and strip deformation leading to buckling

The roll load profile F(y) computed by the coupled roll / strip deformation model is pictured

in Fig. 2a, together with the resulting shape of the deformed roll generator (Fig. 2b). By the

way, Fig. 2b illustrates the very weak effect of coupling or not buckling on these in-bite

characteristics.

The work roll shape displays a large flattening component, of the order of 0.07 mm. The

bending component shows outside the work roll / strip contact (i.e. y > 430 mm), and is partly

hidden in the contact area by flattening. The roll load profiles display distinct peaks near the

edge of the strip for the work roll and at the edge of the work roll for the backup roll. The

peak of the work roll load profile is explained by Fig. 3, which shows that the reduction, from

a nominal, central 29%, reaches 50% at the very edge of the strip, with a significantly longer

bite.

12

0

2000

4000

6000

8000

10000

12000

14000

16000

F( y)

(k N

y (mm)

Zr ol

l ( m

Fig. 2 Coupled deformation of strip and roll:

(a) work roll (WR) and backup roll (BUR) load profiles F(y)

(b) roll generator shape, comparing calculations with / without accounting for strip buckling

0,15

0,17

0,19

0,21

0,23

0,25

0,27

0 50 100 150 200 250 300 350 400 450

Width coordinate y (mm)

0 50 100 150 200 250 300 350 400 450

Width coordinate y (mm)

Th ic

kn es

s re

du ct

io n

(a) (b)

Fig. 3 Strain heterogeneity. (a) comparison of inlet and exit strip thickness profiles. (b) the

thickness reduction profile

4.3 Impact of buckling being accounted for

With a reservation for very small reduction (temper-rolling), it has been found that this

rearrangement of out-of-bite stress has significant impact neither on strain and stress fields in

13

the bite, nor on the roll loads and deformation [1]. Neglecting buckling is therefore licit if

only the behaviour in the bite is to be studied.

Fig. 4 Comparison of the experimental and numerical σxx(y) stress profiles, ≈ 1 m after roll

bite exit

But the “residual” stress field in the strip, under these conditions, is very far from the flatness

roll measurement, as shown in Fig. 4. “Residual” means here post-bite, on-line under tension.

The measurements (dots) show an almost flat stress profile (at the scale of the drawing). FEM

results without buckling (dashed line) give an enormous compressive stress at the edge, due

to a very large elongation gradient connected with roll flattening and the edge drop defect

(see Fig. 3). This very high compressive stress is compensated for by a high tensile stress in

the centre, since the resultant must be equal to the sheet tension force (here given by the

tension stress of 100 MPa, Table 1). Also to be noted is a stress peak at y ≈ 415 mm (i.e. ca.

10 mm from strip edge). It is much more conspicuous when buckling relaxes partly the stress

14

(as in figure 8 or 12); the same location and amplitude is found whatever the mesh size; it is

in fact exactly at the location where the edge-drop starts, i.e. the transition between the

flattened and free zones of the roll profile, see figure 2b.

When buckling is accounted for, i.e. equations (1-4) are activated, the computed stress profile

(full line) comes close to the experiments. More details can be found in the authors’ previous

paper [1]. Therefore, for out-of-bite stress prediction and comparison with stress-meter

measurements, accounting for buckling is essential, at least for thin strips.

a b

Fig. 5 σxx stress maps at the edge, in the vicinity of the roll bite. a - without buckling

computation. b - with buckling computation. Rolling direction Ox is vertical, upward.

Fig. 5 shows the σxx stress map at the edge, slightly before and slightly after the roll bite, i.e.

far ahead of the location of the profiles of Fig. 4. It compares computations without (Fig. 5a)

and with (Fig. 5b) the buckling model. The stress is very much compressive in the bite as

15

expected. In the latter case, a thorough reorganization of the stress pattern just after bite exit

results in the stress being relaxed to almost zero on the edge within 20 – 30 mm from bite exit,

instead of dropping abruptly to -1200 MPa.

a b

Fig. 6 « Buckling strain » principal components: a - λI (corresponding to σxx stress); b - λII

(corresponding to a σyy stress)

Fig. 6 maps the λi’s in the same area. It is found that the reference and principal stress frames

coincide almost everywhere, i.e. α = 0, except for small high shear zones at the edge on either

sides of the roll bite. Hence λI ≠ 0 corresponds to a x-wave (wavy edge) and λΙΙ ≠ 0 to y-wave,

the so-called “towel effect”. Whereas the former is moving with the strip and constitutes a

real flatness defect, the latter is a stationary phenomenon which can be observed sometimes at

the exit of the bite. It is due to a flexible membrane being submitted to a tension under a non-

strictly homogeneous tension stress (e.g. due to the clamping effect of the roll bite). It has no

practical consequences for the strip most of the time, except if it becomes so large that double

thickness rolling occurs; this improbable case is not addressed here.

16

Both types of waves are detected by the model. It should be emphasized, though, that the

present buckling model is embedded in a steady state rolling model, so that it represents a

moving defect in a stationary context. It can therefore detect wave formation, but not

characterize its geometry.

5. FIRST APPLICATION: IMPACT OF TEMPERATURE FIELD ON FLATNESS

Most of the time, thermal effects are neglected in steel cold rolling, and flatness defects are

studied under isothermal conditions. Here, with all three couplings available: strip – roll,

mechanical - thermal, and buckling, many effects may be investigated.

Indeed, at bite exit, the temperature is much larger at the edge than in the centre (Fig. 7),

about 438 K (165°C) versus 383 K (110°C). This is due to larger reduction and plastic

heating (see Fig. 3). Due to the corresponding differential dilatation, the post-bite stress

pattern could be affected. A series of simulations has therefore been run, with roll

temperature calculated at steady state (i.e. after a long rolling time). The isothermal case is

taken as a reference. In the second case, the strip is allowed to cool after bite exit under the

effect of the strip cooling system, with heat transfer coefficient (HTC) Hcool = 5 kW.m-2.K-1 ;

strip - roll contact is kept adiabatic (Hroll = 0). Temperature increases in the roll bite and

slowly decays afterwards (remember 1 m ≈ 0.05 s). In the third case, the roll - strip interface

is represented by Hroll = 100 kW.m-2.K-1. The temperature increase is less in the bite, cooling

is similar to the previous case. Finally, in the fourth case, Hcool = 5 kW.m-2.K-1, Hroll = 100

kW.m-2.K-1, but rolls are moreover cooled efficiently by water sprays, so that strip

temperatures are significantly lower.

Yet, the temperature difference between strip edge and centre is very similar in all 3 cases,

313 to 323 K (40°C to 50°C). Fig. 8 shows that these temperature differences, even in the

17

isothermal case (T = 298 K or 25°C everywhere), have negligible impact on the stress pattern

once relaxed by edge buckling.

Fig. 7 Effect of thermal boundary conditions on central and edge longitudinal temperature

profiles in the rolled strip. Top: long range post-bite evolution. Bottom: detail of plastic

heating in the roll bite

18

Fig. 8 Effect of all thermal boundary conditions on stress transverse profile, σxx(y)

6. FRICTION-SENSITIVE SETTING OF WORK ROLL BENDING FORCES

Work roll bending is a typical sheet profile and flatness actuator: by applying a torque

opposed to the contact stress moment, rolls are brought closer to their rest shape. This is a

more flexible actuator than e.g. roll crown, which is chosen and fixed for a whole roll

mounting. The work roll bending force can be controlled by monitoring the post-bite strip

stress profile by a flatness roll, to answer variations in rolling conditions. Such variations

often come from friction which may fluctuate due to (i) progressive roll roughness wear from

coil to coil or (ii) accelerations and decelerations at coil beginning and end. Jiang and co-

workers have proved in [19] that friction impacts strip profile after cold rolling and

demonstrated the effect of a parabolic variation of friction in the transverse direction in [20].

It is therefore important to quantify the effects of such friction time variations. Friction is

assumed homogeneous here.

6.1 Impact of friction on roll deformation

Figs. 9-12 illustrate a parametric study whereby friction varies between µ = 0.01 (slight

skidding) and µ = 0.035. The impact on roll deformation under a fixed work roll bending

force of 482 kN is first shown. Low friction gives a low rolling load (Fig. 9), and moderate

roll deformation (Fig. 10). The shape of the work roll generator therefore mainly corresponds

to counter-bending by the work roll bending force.

Fig. 9 Effect of varying friction on the work rolls load profile F(y). Work roll bending force

is equal to 482 kN

At µ = 0.035, the rolling load is very high (compare the work roll load profiles), so that roll

kiss occurs (work rolls touch each other on either sides of the strip). The resulting strip

thickness profiles show differences (a few µm) which may look small, but are very important

in terms of residual stress and flatness. The latter are pictured in Fig. 12: µ = 0.01 gives

strong tension on edges and slack centre (wavy centre), whereas the stress profile is most flat

when µ = 0.03, leaving just a few mm of slack metal near the edges, with a probable small

size wavy edge there.

20

Fig. 10 Effect of varying friction on the deformed roll generator shape (bottom). Work roll

bending force is equal to 482 kN

Fig. 11 Effect of varying friction on strip thickness profile (bottom). Work roll bending

force is equal to 482 kN

21

Fig. 12 The impact of friction and transverse profile of strip stress (latent flatness defect).

Work roll bending force is equal to 482 kN

6.2 Impact of work roll bending force at fixed µ

Now, the work roll bending force is varied at constant µ = 0.025 (Fig. 13). The very high

work roll bending force (900 kN) again gives a low, yet positive, stress in the centre, which

will probably result in a wavy centre, at least after tension is cancelled. The most flat stress

profile turns out to be for a work roll bending force equal to 350 kN.

Finally, Fig. 14 summarizes the bending force found “optimal” for each value of the friction

coefficient, i.e. giving the most flat stress profile “by eye”. This graph gives an idea of how to

preset the work roll bending force as a function of varying friction, in the present rolling

operation of Table 1.

22

Fig. 13 The σxx(y) stress profile for varying bending force and fixed friction coefficient µ =

0.025

Fig. 14 The relationship between friction and optimal bending force

23

7. CONCLUSION

The main outcome of the present paper is to show that a simple buckling model can be

coupled to a finite element rolling model and applied to practical questions concerning

flatness in cold strip rolling. In-bite stress and strain are not affected by post-buckling stress

rearrangement, but the residual stress is, in case of manifested defects expected with very thin

strips.

The results presented above suggest that for cold rolling, the heterogeneous temperature field

does not change significantly the stress pattern, which is dominated by the rearrangement of

the stress field as the elastic strain recovery takes place in the immediate post-bite area. This

analysis contributes to shed light on which features of the rolling process may be neglected or

not, depending on the objective: in bite stress and strain, roll deformation and strip crown do

not need particularly buckling to be coupled; the residual state of the strip is very sensitive to

buckling whenever it takes place on-line, but it is not sensitive to thermal transfer.

It has been shown also here that friction has an impact on reduction profile, in particular on

the edge thickness, through roll load distribution and roll deformation. This strongly changes

residual stress distribution when thin strips are dealt with. For a given work roll bending force,

just changing friction may turn the strip shape from flat to wavy edge to wavy centre.

Conversely, for each level of friction, an “optimal” work roll bending force can be proposed

based on results of the model.

The buckling model presented in section 3.2 deals with buckling at material point (or finite

element) level, which is questionable; but it is strongly coupled at constitutive equations level,

which Abdelkhalek et al. have shown to be important for precise residual stress prediction

[21]. It cannot predict the geometry of defects quantitatively. These are serious limitations.

24

Work is in progress to try and implement more physically founded models which give

quantitative information on defect geometry. These efforts will be reported somewhere else.

ACKNOWLEDGEMENT

The authors wish to thank the French National Research Agency (ANR) for its financial

support under Contract ANR – 2010- RMNP-019-01, and the partners of the Platform Project

(ArcelorMittal Maizières research, Constellium CRV, CNRS, CEA, Université de Lorraine,

INSA Lyon and ARMINES) for authorization to publish this work. Particular thanks are due

to M. Potier-Ferry and H. Zahrouni, from LEM3 laboratory, for most helpful discussions.

REFERENCES

1. Abdelkhalek S, Montmitonnet P, Legrand N, Buessler P (2011) Coupled approach for

flatness predictions in thin strip cold rolling. Int. J. Mech. Sci. 53: 651-675

2. Timoshenko S, Woinovsky-Krieger S (1940) Theory of plates and shells, McGraw-Hill

Book Co., New York

3. Bush A, Nicholls R, Tunstall J (2001) Stress levels for elastic buckling of rolled strip

and plate. Ironm. Steelm. 28: 481-484

4. Fisher FD, Rammerstorfer FG, Friedl N, Wisser W (2000) Buckling phenomena related

to rolling and levelling of sheet metal. Int. J. Mech. Sci. 42: 1887-1910

5. Yukawa N, Ishikawa T, Tozawa Y (1986) Numerical analysis of the shape of rolled

strip. In: Proc. NUMIFORM Conference, August 25-29, Gothenburg, Sweden

6. Abdelkhalek S, Zahrouni H, Potier-Ferry M, Montmitonnet P, Legrand N, Buessler P

(2009) Modélisation numérique du flambage des plaques minces et application au

laminage. In : Proc. (CD-ROM) CFM 2009August 24-28, Marseille, France. In French

25

7. Zahrouni H, Cochelin B, Potier-Ferry M (1999) Computing finite rotations of shells by

an Asymptotic-Numerical Method. Comp. Meth. Appl. Mech. Engg 175: 71-85

8. Boutyour EH, Zahrouni H, Potier-Ferry M, Boudi M (2004) Bifurcation points and

bifurcated branches by an Asymptotic Numerical Method and Padé approximants. Int.

J. Num. Meth. Engg, 60: 1987-2012

9. C. Counhaye (2000) Modélisation et contrôle industriel de la géométrie des aciers

laminés à froid. PhD Thesis, Liège University. In French

10. Roddeman DG, Drukker J, Oomens CWJ, Janssen JD (1987) The Wrinkling of Thin

Membranes: Part I-Theory. ASME Trans. J. Appl. Mech. 54: 884-887

11. Hacquin A (1996) Modélisation thermomécanique tridimensionnelle du laminage -

Couplage bande / cylindres (3D thermomechanical model of rolling - Strip-roll

coupling). PhD Thesis, Ecole des Mines de Paris, France. In French.

12. Hacquin A, Montmitonnet P, Guilleraut JP (1998) A steady state thermo-elasto-

viscoplastic finite element model of rolling with coupled thermo-elastic roll

deformation. J. Mat. Proc. Tech. 60: 109-116

13. Hacquin A, Montmitonnet P, Guilleraut JP (1998) A 3D semi-analytical model of

rolling stand deformation with finite element validation. Eur. J. Mech. A (Solids) 17:

79-106

14. Berger B, Pawelski O, Funke B (1976) Die elastische Verformung der Walzen von

Vierwalzengerüsten. Arch. Eisenhüttenwes. 47: 351-356. In German

15. Hacquin A, Montmitonnet P, Guillerault JP (1994) Experimental validation of a Rolling

Stand Elastic Deformation Model, J. Mater. Process. Technol. 45: 199-206

16. Montmitonnet P (2006) Comparison of profile prediction models for strip rolling,

Conference “Achieving Profile & Flatness in Flat Products” Austin Court, Birmingham,

UK

26

17. J. Yanagimoto , M. Kiuchi : 3D simulation system for coupled elastic / rigid plastic

deformation of rolls and workpieces in strip rolling processes. Proc. NUMIFORM 92

(Sophia-Antipolis, France, 1992). J.L. Chenot et al. eds. A.A. Balkema, Rotterdam

(1992)

18. T.H. Kim, W.H. Lee, S.M. Hwang : An integrated FE process model for the prediction

of strip profile in flat rolling. ISIJ Int. 43, 12 (2003) 1947-1956

19. Jiang ZY, Tieu AK, Zhang XM, Lu C, Sun WH (2003) Finite element simulation of

cold rolling of thin strip. J. Mat. Proc. Tech. 140: 542–547

20. Jiang ZY, Xiong SW, Tieu AK, Wang QJ (2008) Modelling of the effect of friction on

cold strip rolling. J. Mat. Proc. Tech. 201: 85-90

21. Abdelkhalek S, Zahrouni H, Montmitonnet P, Legrand N, Potier-Ferry M (2011)

Manifested flatness predictions in thin strip cold rolling using a general rolling FEM

model, Steel Res. Int., Sp. Iss. “ICTP 2011” :111-116

27

Figure captions

Fig. 1 Schematic view of flatness defects. Note reference frame : x = Rolling Direction

(RD), y = Transverse Direction (TD), z = Normal Direction (ND)

Fig. 2 Coupled deformation of strip and roll:

(a) work roll (WR) and backup roll (BUR) load profiles F(y),

(b) roll generator shape, comparing calculations with / without accounting for

strip buckling

Fig. 3 Strain heterogeneity. (a) comparison of inlet and exit strip thickness profiles. (b)

the thickness reduction profile

Fig. 4 Comparison of the experimental and numerical σxx(y) stress profiles, ≈ 1 m after

roll bite exit

Fig. 5 σxx stress maps at the edge, in the vicinity of the roll bite. a - without buckling

computation. b - with buckling computation. Rolling direction Ox is vertical,

upward.

Fig. 6 « Buckling strain » principal components: a - λI (corresponding to σxx stress); b

- λII (corresponding to a σyy stress)

Fig. 7 Effect of thermal boundary conditions on central and edge longitudinal

temperature profiles in the rolled strip. Left: long range post-bite evolution.

Right: detail of plastic heating in the roll bite

Fig. 8 Effect of all thermal boundary conditions on RD stress transverse profile, σxx(y).

Fig. 9 Effect of varying friction on the work rolls load profile F(y). Work roll bending

force is equal to 482 kN

Fig. 10 Effect of varying friction on the deformed roll generator shape (bottom). Work

roll bending force is equal to 482 kN

28

Fig. 11 Effect of varying friction on strip thickness profile (bottom). Work roll bending

force is equal to 482 kN

Fig. 12 The impact of friction and transverse profile of strip stress (latent flatness

defect). Work roll bending force is equal to 482 kN

Fig. 13 The σxx(y) stress profile for varying bending force and fixed µ = 0.025)

Fig. 14 The relationship between friction and optimal bending force

Table caption